Embed Size (px)
Transcript of Biopolymer-ZnO nanocomposite
Multifunctional ZnO-Biopolymer Nanocomposite Coatings for Health-Care Polymer Foams and FabricsP. K. Sanoop,1 K. V. Mahesh,1 K. M. Nampoothiri,2 R. V. Mangalaraja,3 S. Ananthakumar11 Nanoceramics Division, National Institute for Interdisciplinary Science and Technology, Council of Scientific and Industrial Research (CSIR), Thiruvananthapuram, Kerala 695019, India 2 Biotechnology Division, National Institute for Interdisciplinary Science and Technology, Council of Scientific and Industrial Research (CSIR), Thiruvananthapuram, Kerala 695019, India 3 Department of Engineering Materials, University of Concepcion, Concepcion, Chile
Received 5 August 2011; accepted 16 January 2012 DOI 10.1002/app.36831 Published online in Wiley Online Library (wileyonlinelibrary.com). ABSTRACT: Biopolymer-mediated sonochemical synthesis has been carried out for obtaining stable, nanocrystalline ZnO-biopolymer nanocomposite colloids to be applied on polymer foam and cotton fabrics to ultimately produce multifunctional, heath-care surface modifications. In situ nucleation and growth of nano-ZnO was achieved by ultrasonication at $ 60 C in aqueous biopolymer media prepared using starch, gelatin, chitosan, and agar. Phase analysis, structurebonding characteristics, ZnO morphology, particle size distributions, rheology, and thermal decompositions were studied using XRD, FTIR, SEM/ TEM, viscometer, and TG/DTA tools. Morphologically varied nanocrystalline ZnO of size $ 40 nm were synthesized. Biopolymers media resulted in stable ZnO colloids through steric stabilization. ZnO-biopolymer nanocomposites colloid was applied on polyurethane foams and cotton fabric substrates by dip coating. These coatings were examined for the UV photoactivity and resistance to fungi growth. A comparison has been made among the biopolymers. It is shown that the surface coatings of ZnO-biopolymer nanocomposites can produce anti-fungal, UV active polymer foams and fabrics. The study has significant relevance in automobile and hospital industries because such functionally modified polymer foams and cotton fabrics can be disinfected and refreshed just by periodic applicaC tion of water-free, UV cleaning. V 2012 Wiley Periodicals, Inc.J Appl Polym Sci 000: 000000, 2012
Key words: biopolymers; coatings; polyurethanes; surface modification
INTRODUCTION Applications of nano-engineered inorganic-polymer hybrid soft-coatings on the surfaces of textiles, leather, and home appliances received wide popularity because they offer attractive multifunctional properties like oil-repellent, stain-free, self-cleaning surfaces, photoactive decomposition against organic pollutants, and most importantly resistance to moisture and moist-air penetration characteristics. The polyurethane foam surfaces are hydrophobic and naturally resist the moisture. However, in many practical or service conditions, over a period of time, especially when they are exposed to rainy and high humidity atmospheres, as well as indoor conditions having wet atmosphere and improper ventilations, every chance is there for the fungus to grow. Nanometric oxides like TiO2, SiO2, and ZnO and their hybrids are found successful to produce hydro-
Correspondence to: S. Ananthakumar (ananthakumar70@ gmail.com).C V 2012 Wiley Periodicals, Inc.
Journal of Applied Polymer Science, Vol. 000, 000000 (2012)
phobic, eco-friendly functional coatings.13 Hydrophobic nature is particularly important in textiles because cottons and synthetic textiles build up static charges due to moisture. Cotton textile fabrics are porous in nature and readily absorb moisture in humid conditions. The moist-air favors bacteria and fungus growth which in turn causes severe breathand skin-related health hazards. Organization like Cotton Research Institute in India has been developing health-care functional coatings on textiles using TiO2, ZnO, and SiO2 hybrids. In addition to the antimicrobial, antifungal, and antistatic characteristics, they also offer UV-blocking property.46 UV shielding sunscreen surface coatings on textiles help to protect human skin from sun burn and skin-cancer. Nano TiO2/Ag, ZnO/SiO2/polyester hybrids, and ZnO-starch composites are being tested as UV shielding textile coatings. ZnO/TiO2 nanocomposites are better candidate for UV active self-cleaning surface coatings. Concerning the photoactivity, TiO2 is more effective only when the TiO2 precursor coatings are heat treated at $ 400 C.7,8 It complicates more to adopt the UV-active TiO2 coatings for soft surfaces like textiles. Functional nanoZnO has advantages over TiO2 because ZnO can block
SANOOP ET AL.
UV in the entire ranges (UV-A, UV-B, and UV-C). It also exhibits antibacterial property in neutral pH even with low quantity of ZnO. Moreover unlike TiO2 nanoparticles, the ZnO nanocrystals can be easily grown by varieties of chemical techniques at mild synthesis conditions using cheap precursors. ZnO nanoparticles in different morphologies ranging from rods, tubes, discs, spheres to wires, and arrays have been easily synthesized by surfactantassisted precipitation followed by low temperature thermolysis ($ 80 C) and hydrothermal processes ($ 120 C).913 Surfactant-assisted synthesis has claimed monodisperse nano-ZnO with particles diameter < 10 nm.14 Encapsulation of ZnO precursor in biopolymer media followed by mechanical activation is an efficient technique to generate in situ nucleation and growth of nanocrystals. This has been attempted in this work for obtaining size and shape controlled nano-ZnO through biopolymermediated sonochemical technique. The high energy chemistry explains the mechanism involved in the sonochemical technique. Accordingly, the formation and growth of gas bubbles takes place first, which occurs through the diffusion of solute vapor to the volume of the bubble. When the size of the bubble reaches a maximum value it collapses. The collapse of bubbles in a multibubble cavitation field produces hot spots with effective temperatures of $ 5000 K, pressures of $ 1000 atmospheres, and heating and cooling rates above 1010 K/s. These extreme conditions are favorable for the nucleation and growth of the nanoparticles.15 Polymer foams are usually hydrophobic and physical binding of inorganic nanoparticles with foams is ensured by adhesive nature of the biopolymers. The incorporation of biopolymer is only